Embed Size (px)
Table of Contents
Abstract ................................................................................................ 1
1 Introduction ......................................................................................... 1
2 Hopping Conduction .......................................................................... 2
2.1 Deviations from coulomb gap behavior ....................................... 3
2.2 Doping and device fabrication .................................................... 6
Neutron transmutation doped germanium ................................. 6
Ion-implanted silicon ............................................................... 6
3 Electrical Nonlinearities ...................................................................... 10
3.1 Electric field effects ..................................................................... 10
3.2 “Hot electron” effects ................................................................... 10
Time constants and heat capacity ............................................. 15
Internal thermodynamic fluctuation noise ................................. 15
4 Excess noise ...................................................................................... 16
5 Fundamental Limitations and Ultimate Performance .................... 21
5.1 Optimization ................................................................................ 22
5.2 Germanium vs Silicon ................................................................. 22
5.3 Expected performance ................................................................ 23
References .............................................................................................. 25
Physics Department, University of Wisconsin, Madison, WI 53706 USA
Abstract. Semiconductor thermistors operating in the variable range hopping conductionregime have been used in thermal detectors of all kinds for more than fifty years. Theiruse in sensitive bolometers for infrared astronomy was a highly developed empirical arteven before the basic physics of the conduction mechanism was understood. Today weare gradually obtaining a better understanding of these devices, and with improvementsin fabrication technologies thermometers can now be designed and built with predictablecharacteristics. There are still surprises, however, and it is clear that the theory of theiroperation is not yet complete. In this chapter we give an overview of the basic operationof doped semiconductor thermometers, outline performance considerations, givereferences for empirical design and performance data, and discuss fabrication issues.
1 IntroductionEarly thermal detectors were hampered by the lack of practical thermometers with goodsensitivity at low temperatures. Thermocouples and metallic resistance thermometersrapidly lose sensitivity below room temperature. Semiconductor thermistors were in useat high temperatures, but the readily available semiconductors — mostly metal oxides —became much too resistive when cooled. All of the most sensitive devices discussed inR. Clark Jones' classic 1947 paper on the ultimate sensitivity of thermal detectorsoperated at room temperature .
By 1950 there were conference reports indicating that doped germanium could be asuitable thermometer at temperatures as low as 1 K , but reproducibility was elusive.Material purity and characterization were difficult issues, and providing low-noiseelectrical contacts was a poorly understood black art. By 1961, Frank Low haddeveloped practical gallium-doped germanium devices operating at liquid heliumtemperature with noise equivalent power (NEP) below 10–12 W/Hz1/2 . The radiofrequency resistivity of this material made it a reasonable match to free space, so thesensing element could also be used as an efficient radiation absorber, and these“germanium bolometers” were soon applied to the burgeoning field of infraredastronomy.
Today, developments by the semiconductor electronics industry have solved many of thematerials and fabrication issues. Germanium and silicon are readily available with morethan adequate purity, essentially noise-free contacts are easily formed by ion-implanteddoping, and a host of techniques and machines are available that facilitate the fabricationof the thermistors, thermal isolation structures, and large arrays of detectors and theirelectrical interconnections. There have been considerable advances in theoretical
understanding of the conduction mechanism. As we will see below, this understanding isfar from complete, but empirical characterizations should be adequate for optimizing thedesign of low temperature detectors, and for predicting their ultimate performance withthermometers of this type.
2 Hopping Conduction
Shallow impurities in germanium and silicon have binding energies typically tens ofmilli-electron volts and are almost completely ionized at room temperature. As thetemperature is lowered, the ionized fraction drops rapidly. This produces an increase inthe resistance of lightly-doped material, but for most low temperature thermometryapplications this is not the regime nor mechanism of interest. Instead, we are normallyworking at temperatures where thermal ionization of impurities is negligible. While thecrystal structure is perfectly regular, the random substitution of dopant atoms at a smallfraction of the lattice sites produces a disordered system that has, at sufficiently lowtemperatures, the electron transport properties of an amorphous material. The basicproperties of such systems were determined by Anderson  and Mott . They findthat there is a critical doping density below which the conductivity goes to zero at zerotemperature, and above which there is always a finite conductivity. We are interested inmaterials doped below this “metal-insulator transition”, where charge transport takesplace by phonon-assisted tunneling between impurity sites. The energy levels of thesesites are effectively randomized by the long-range coulomb potential of chargesdistributed over distant sites, and the energy difference required in a given tunnelingevent or “hop” is made up by absorption or emission of a phonon of the required energy.
At sufficiently high temperatures, the distance barrier wins and hops take place to thenearest unoccupied site. This is referred to as “nearest neighbor hopping”. At lowertemperatures, the scarcity of high energy phonons favors longer hops as necessary to findan unoccupied site sufficiently close to the same energy that a phonon is more readilyavailable. This is usually the regime of interest for low temperature thermometry, and theprocess is called “variable range hopping” (vrh). An extensive development of the theorycan be found in the text by Shklovskii and Efros . For vrh, the conduction is expectedto behave as
R T RT
( ) exp=⎛
0 , (1)
where Mott found p = 1/4 for the approximately constant density of states he expected atthe fermi level. Efros and Shklovskii later showed that the changing coulombinteractions accompanying a hop should guarantee the existence of a parabolic gap in thedensity of states centered at the fermi level . This modifies the result to make p = 1/2.
Measurements at the time, particularly on germanium and silicon, usually did not lookmuch like this. Experiments gave a variety of R(T) curves that were not reproduciblefrom one sample to the next. However, data from samples doped by nucleartransmutation (NTD) or by careful ion implantation do show the expected behavior. Thiscan be seen in Fig. 1, where the T–1/2 behavior predicted by vrh with a “coulomb gap” isquite accurately followed over several orders of magnitude in resistance.
Even modern melt-doped material seldom shows this clear coulomb gap behavior. Theresistance usually flattens as the temperature is reduced, and the power-density effectsdiscussed below become apparent at lower than expected power levels. Both of theseobservations are consistent with the existence of small-scale nonuniformities in thedoping density, but it is not clear that this is the correct explanation.
2.1 Deviations from coulomb gap behavior
At sufficiently low temperatures, when T0/T > ~24, systematic deviations from thiscoulomb gap behavior are observed [8,9]. This is shown in Fig. 2, where R(T) is plottedfor ion-implanted silicon samples with several different doping densities. It is clear thatmany of these curve upwards, but it is difficult to see a pattern in the deviations and infact would be difficult to detect them at all had the lowest temperatures been included inthe straight line fits. However, if we divide out the coulomb gap model fits, wherelog /R T∝ −1 2 , and plot the ratio as a function of the temperature normalized by T0 for eachsample as shown in Fig. 3, it can be seen that the deviations are quite systematic.
Shlimak observed similar behavior in arsenic-doped germanium, and suggested that amagnetic hard gap due to spin-spin interactions might be responsible . There isevidence that R(T) reverts to coulomb gap behavior with applied magnetic fields > 1 T,which supports the idea that the deviations are some kind of magnetic effect .
From an experimental standpoint, this low-temperature rise can easily be masked by lightleaks, RF pickup, or other extraneous heating effects, all of which tend to makemeasurements turn down below the intrinsic R(T) curve. It is useful to have an analyticexpression that can be fit to measurements at higher temperatures, where these effects are
Fig. 1. Measured R(T) for ion-implanted silicon. The linear dependence of log(R) on T–1/2
predicted by the variable range hopping model with a coulomb gap is observed over severalorders of magnitude in resistance
0 0.5 1 1.5 2
0 1 2 3 4 5
1.4 K4.4 K8.3 K 19 K 28 K 48 K
T (K)1.010 0.3 0.1 0.05
fit = 0 exp(T0/T)
usually negligible, and extrapolated to compare with the lowest temperaturemeasurements to determine the extent of any heating problems. Of course, it is alsoconvenient for thermometric purposes to have such a function, since only a small numberof calibration points are then required to fix the entire R(T) dependence. Wouter
Fig. 2. Resistivity vs T–1/2 for six ion-implanted Si:P,B samples. The different samples havedifferent doping densities, which determines the value of T0 in (1). The straight lines are fits tothe coulomb gap model over a temperature range 6.5 < T0/T < 24. (from )
Fig. 3. Resistivity of samples in Fig. 2 divided by the best-fit coulomb gap model vs thenormalized inverse temperature T0/T. (from )
Bergmann-Tiest has fit the deviations with a purely empirical function, which isreproduced here :
R T RT
T( ) exp exp=
⎠⎟ + ′
where ′ = −−R R T0 0 00 252 522 8 733exp( . . ). and ′ = +T T0 02 7148 1 2328. . .
This is not pretty, but it introduces no additional free parameters, and considerablyincreases the temperature range over which a good fit can be made. (In principle, thereshould be only one free parameter to the fit, which is T0 and corresponds to the dopingdensity. R0 should be calculable from this and the sample geometry. In practice howeverthis cannot be done with the required precision, so R0 is normally fit simultaneously).The function is designed to give the same values for R0 and T0 as the coulomb gap modelif the latter is fit only to the higher temperature data.
The generality of whatever effect is producing this low-temperature deviation isillustrated in Fig. 4, which shows R(T) for an NTD germanium sample, fit by both thesimple coulomb gap model and by the “Wouter function” given above. Each has thesame two free parameters The Wouter function was derived from the behavior of verythin (0.3 µm) ion-implanted silicon samples, but it provides a good fit for this relativelythick (200 µm) NTD germanium device.
0 1 2 3 4 5
VRH (Linear) fit
10 1 0.3 0.1 0.05T (K)
NTD GeT0 = 4.45 K
Fig. 4. Resistance of a 200 x 1000 x 2000 µm3 NTD germanium thermometer, showing thebest-fit coulomb gap model and a fit using the “Wouter function” given in (2). The fixedparameters of this function were derived from a set of thin ion-implanted silicon samples.Both functions were fit only to data for 4K < T < 0.2K
This function works reasonably well, but its additive term offers little help with physicalsignificance. Laura Rose Semo-Sharfman has made another fit to similar data, and choseto represent the correction as a multiplicative term :
R T RT
( ) exp=⎛
⎠⎟ ⋅ +
01 . (3)
where A T B= − ⋅ −( . . ln )0 1884 0 01241 600 and B T= + −2 074 3 179 8 810. . exp( / . ). Thisactually doesn’t fit quite as well as (2), but it is well within the systematic accuracy of thedata. Woodcraft et al.  use a variable value of p in (1) instead, but this gives poor fitsto the data in .
2.2 Doping and device fabrication
This section contains quantitative information on doping germanium and silicon fordevice thermometers, and some examples of construction techniques.
Neutron transmutation doped germanium. Extremely reproducible thermometers canbe produced by irradiating germanium with reactor neutrons . Natural germaniumhas four stable isotopes with substantial abundances, and the neutron cross sections andabundances of two of these conspire to produce gallium-doped (p-type) material that is32% compensated with arsenic. Since the isotopes are chemically identical, they arepresumably distributed perfectly randomly in the lattice, and the moderate neutron crosssection makes the neutron flux uniform throughout even quite large blocks ofgermanium. These can then be cut up to make large numbers of very uniformthermometers. Plots of the resistivity ρ(T) for a number of different neutron doses areshown in Fig. 5, and the fit T0 vs net doping density is given in Fig. 6. The value of ρ0
should also be a simple function of doping density, and a plot of this is given in .However, the derived value is highly correlated with the T0 fit, small systematic problemswith the data make large differences, and there is little agreement in published values.Inspection of Fig. 5 shows that over a wide range of intermediate values of T0, ρ0 iswithin a factor of ~2 of 0.1 ohm cm, while samples with extreme values of T0 can be afactor of 100 or more different.
The uniformity and predictability of NTD Ge thermometers is particularly valuable in theconstruction of large arrays of detectors. However, the penetrating power of the neutronsthat helped provide the very uniform doping also means that it is impractical to mask theprocess and dope only selected areas in a crystal. So the thermometers must be cut to theoptimum dimensions, and then individually attached to the detector elements. This is nota drawback, however, when the elements are very large and individually mounted, as inthe CUORE project . For arrays of small detectors, clever use of hybrid circuitmounting techniques that treat the thermistors as components to be “bump-bonded” canallow the use of integrated wiring and somewhat automated assembly .
Ion-implanted silicon. Silicon requires very large neutron doses to dope bytransmutation, and this is seldom attempted. However, doping by implanting ions from abeam with kinetic energies from tens of keV to a few MeV is a well-developed techniquein the semiconductor electronics industry. This allows penetration depths of up to ~1 µm,
but results in an approximately Gaussian density profile with depth. Uniform densitiescan be obtained by superimposing implants with several different energies and carefullydesigned doses to produce a flat-top profile [8,9], or by implanting a single dose of eachion into a thin piece of silicon, preferably capped with SiO2 on both sides, and thentreating it at high temperature to allow the implanted ions to diffuse completely and
Fig. 6. Doping density parameter T0 vs net doping density ( )n nacceptor donor− for neutron
transmutation doped germanium. Data provided by 
0 5 10 15 20
T 0 (
nd = 0.285 na (28.5%)
nd = 0 (uncompensated)
T0 = 430 (1 – n/nc)2, nc = 2.7 × 1017
T0 = 112 (1 – n/nc)2, nc = 8.7 × 1016
Net Doping Density n na – nd (×1016 cm–3)
Fig. 5. Resistivity vs temperature for a number of samples of transmutation dopedgermanium exposed to different neutron fluences 
Resistivity of NTD Germanium
2 4 5
0 1 2 3 4 5 6 7 8
500 300 200 100 50 40 30 25 20 16
uniformly throughout the thickness . The diffusion times and temperatures arepractical up to a thickness of a few microns.
The great advantage of this doping method is that it can be masked by standardphotolithographic techniques, allowing the simultaneous fabrication of large numbers ofthermistors than can have almost arbitrarily small dimensions, and have fully integratedelectrical connections [21,22]. Silicon also has excellent mechanical and thermalproperties, and many techniques exist for fabricating mechanical structures from it thatcan be used, for instance, for thermal isolation of the individual detector elements. Fig. 7shows a sketch of the structure for a single pixel of an X-ray detector array, where alimited region is doped to form the thermometer and undoped silicon is used for themechanical structure, including the thermal isolation beam supports. Fig. 8 shows aphotograph of the pixel, and of the entire 6x6 array after the X-ray absorbers have beenattached. Techniques exist that should make it possible to fabricate the absorbersmonolithically, rather than attaching them by hand, but these have not yet been perfected.
Ion implanted thermistors of the stacked-implant variety have been plagued by a lack ofreproducibility that is not understood. Both doses and energies can be measured withmore than adequate precision, but the run-to-run repeatability is poor enough that it iscommon to implant a series of wafers with slightly different doses, and then pick the onethat comes closest to the desired resistivity. Fortunately, uniformity across a wafer isgenerally good, and the steps in implant density within a single processing run give amonotonic sequence. Fig. 9 shows T0 vs doping density for silicon, but it should not betaken too seriously, as the scatter among the data points shows. Diffused thermistorsseem more repeatable, although there is not much experience with them yet.
Fig. 7. Structure of one pixel of a monolithic X-ray detector array with ion-implanted thermistors.
1 1.5 2 2.5 3
T 0 (
T0 = 431 (1 – n/nc)2, nc = 3.38 × 1018
T0 = 577 (1 – n/nc)2, nc = 2.85 × 1018
p-type, 50% compensatedn-type, 5% compensatedn-type, 50% compensated
Net Doping Density n nd – na (×1018 cm–3)
Reference  has a figure showing ρ0 as a function of T0 for implanted silicon. Thedifficulties are the same as for germanium, and this should be regarded as a rough guideonly. The variation seems even smaller than for germanium, however, and ρ0 ≈0.05 ohm cm over a wide range of T0.
Fig. 9. T0 vs net doping density for ion-implanted silicon. Most data are from , but theestimated thickness of these stacked implants has been normalized to results from the smallernumber of diffused samples with accurately determined thicknesses, resulting in a 60%increase in effective thickness and a corresponding reduction in the derived doping densities
Fig. 8. a) One pixel of a monolithic silicon array for the XRS instrument on Astro-E2. Thesmall cylinders on the short curved arms are attach points for the HgTe X-ray absorbers.b) Full view of the 6x6 array after the absorbers are attached with epoxy
3 Electrical Nonlinearities
It might seem that doped semiconductors should make almost ideal thermometers. Thefigure of merit α ≡ d R d Tlog log from Ch. 1 is just α = 0 5 0
1 2. ( )T T for coulomb gapR(T). One can make T0 arbitrarily high by doping lightly, so it should be possible tomake α as large as desired. At the same time, it is easy to fabricate ion-implantedsensors with such small volumes that the heat capacity contribution of the thermometercould be negligible, despite the relatively high specific heat of the doped material.
However, the effects described in this section introduce severe and in most casesfundamental limits to the extent that small volume and high sensitivity can be pursued.None of them is entirely understood theoretically, but empirical data are available (atleast in principle) that allow optimum values for thermistor size and T0 to be determinedfor a given application. These effects also introduce intrinsic limits to the speed ofsemiconductor thermometers.
3.1 Electric field effects
Phonon-assisted tunneling is an inherently non-linear process, and is expected to appearlinear only in the limit of small electric fields. There are several models that differ indetail, but most can be approximated by
R T E R T CeE
kT( , ) ( , )exp ,= −
where E is the electric field, R(T,0) is the resistance in the limit of low fields — thecoulomb gap function in this case — C is a constant of order unity, e is the electroniccharge, and λ is a characteristic hopping length that in most models scales as T–1/2 .See also discussion and references in . This type of behavior is observed in dopedgermanium and silicon under certain conditions [24,25,26], as shown in Fig. 10.
In the linear theory of Ch. 1, this behavior is represented by a local slope β ∂ ∂≡ )R VT
evaluated at the operating point. This is negative, and always acts to reduce thermometersensitivity. Raising T0 by decreasing the doping concentration makes λ larger andincreases the magnitude of this term. To optimize thermometer design, it would be niceto know λ as a function of T0 and T, particularly for NTD Ge, as we will see below.References [24, 25, 26] and  have modest amounts of data for Ge, and less modestamounts of disagreement. This is clearly an area where there is a shortage of neededengineering data.
3.2 “Hot electron” effects
As can be seen in Fig. 11, the standard electric field effect form given in (4) does notalways describe the observed behavior very well. Over most of the parameter range ofinterest for low temperature detectors, field-dependence can be better fit by an analog ofthe hot electron effect in metals [24,28,29]. If the bias power is dissipated in theconduction electron system and sunk through the crystal lattice, one can envision an
0 1000 2000 3000 4000
TSINK = 0.79 K
TSINK = 0.42 K
TSINK = 0.24 KNTD Ge, T0 = 59.4 K
E/T3/2 (Volts m–1 K–1.5)
0 500 1000E/T3/2 (Volts m–1 K–1.5)
Ion-implanted Si, T0 = 4.50 K
TSINK = 0.163 K
Fig. 10. Effect of electric field on resistance for a NTD Ge sample with T0 = 59.4 K at threedifferent heat sink temperatures. The sample was fixed to the sink with a high thermalconductivity. According to (4) with λ∝ T–1/2, the data should follow parallel straight lines.(from )
Fig. 11. As in Fig. 10, but for an ion-implanted Si sample with T0 = 4.5 K , operated at 0.163 K.The solid line is a field-effect model. The dashed line is the hot electron model described in the text
effective thermal conductivity between the electrons and phonons. Again by analogy toother thermal conductivities, this is assumed to have the form G T0
β , making the powertransfer
−( )+ +0 1 1
e lattice . (5)
In such a model, one further assumes that the resistance is a function of Te only. (Notethat this β is unrelated to one used for thermistor voltage dependence.) The R(T)function can be calibrated in the limit of small bias power, where Te ≈ T lattice. Then G0
and β are fit to resistance data taken with a range of bias powers. Figure 12 shows thatthis form fits well over a wide range of electron and lattice temperatures, although β isgenerally found to be ~5, rather than the 4 expected and measured for metals.
Zhang et al  investigated a variety of ion-implanted Si and NTD Ge thermistors witha wide range of doping densities. They found that the difference between the behaviorsof Figs. 10 and 12 is not that one is Ge and the other Si, but is rather the combination ofoperating temperature and doping density. Devices with high T0’s operated at lowtemperatures had behavior well described by the field effect model of (4), while low T0’sand high operating temperatures gave results better represented by the hot electron modelof (5). Thermistors operating near the borderline, roughly described by T T0 100≈ ,didn’t fit either model well.
0.1 1Te (K)
100 101 102 103 104 105 106 107 108
= 0.1 K
T0 = 4.50 KR0 = 2584
Fig. 12. Resistance vs bias power for an ion-implanted Si device. Data series are labeled by latticetemperature. The lines show the hot electron model, with electron temperature derived from (5)and resistance from this Te and (2). The parameters T0 and R0 are fit to measured values of R in thelimit of low power. All data series are fit simultaneously with the same values of G0 and β . Theinset plots G d P V dTe-ph e≡ ( / ) / vs Te, showing a single power-law dependence over four orders of
magnitude in G. (from )
They suggested that both effects were always operative, with one or the other dominatingin most parts of T0-T space, but with both required to explain the behavior in theboundary region, as evidenced by the data shown in Fig. 13 for an Si detector. Piat et al found it essential to use a combined model to fit high quality data on NTD Gethermometers intended for temperature control on the Planck-HFI instrument. Thecombined model simply substitutes Te from (5) for T in the field effect model (4). Themean hopping length λ is assumed to scale as T –1/2, which is observed to be anapproximation at best [24, 25, 26] (and  finds ~T–1), but is adequate for fitting over alimited temperature range.
Like the field effect, hot electron behavior is an important limitation on detectorperformance, and its parameters are needed to optimize detector design. Zhang et al characterized a large number of ion-implanted Si devices with a wide range of dopingdensities. They used the hot electron model to determine values for the electron-phononthermal conductivity parameters G0 and β in (5) as a function of doping density, as shownin Fig. 14. Zhang et al were measuring thin stacked-implant devices, where the effectivethickness is somewhat ambiguous. We have used measurements on a small number ofdiffused implant thermometers, where the thickness is precisely known, to normalize thevolumes used for computing G0/V in Fig. 14b. The devices used for normalization had T0
near 7 K, and the correction was about 40%. It is possible that the correction shouldreally be a function of T0. Also, no corrections were made for electric field effect, whichcould be a significant contributor at the higher T0’s. This would tend to reduce β andincrease G0 in this region.
0 5000 10000
Hot Electron Model
Electric Field Model
E/T3/2 (Volts m–1 K–1.5)
TSINK = TLATTICE = 0.345 KT0 = 60 K
Fig. 13. Data for an ion-implanted Si sample operated near the T0–T borderline that separatesgood fits to the field effect and hot electron models. The solid line shows an electric field effectmodel (4), while the dashed line is for a hot electron model
0 20 40 60
fit = 4.27 + T0/39 K(a)
( P/ Te)|Tph = Ge-ph= G(0.1K)(Te/0.1K)
G(0.1K) = 10(4.04 – 0.0349 T0)
While it is relatively easy to ensure that the lattice temperature remains constant as biaspower is increased with the implanted Si samples, for practical reasons related to thegenerally quite different sample geometry and mounting, this is more difficult for NTDGe. Again because of differences in the usual thermometer geometry, NTD Ge seldomhas useful resistance values where hot electron effects are entirely dominant. Partly dueto these factors, there is less quantitative data available on G0 and β for Ge. References[27, 28] and  have modest amounts of data on this, and again it is not in goodagreement. Piat et al  were the only ones to make a simultaneous fit of the hotelectron and electric field effects, so their results are probably the most reliable.
The difficulty with this “hot electron” model is that it has no basis in current theory ofvariable range hopping conduction. The doping of these devices is far on the insulatingside of the critical density, and the electrons should be strongly localized. The electronscan change their energy distribution by tunneling from site to site, with emission orabsorption of phonons making up the energy difference. But for the electrons to set up athermal distribution of their own independent of the phonons would require that theirenergy be somehow delocalized while the electrons themselves are not . It isinteresting that β = 5 is expected for three-dimensional phonons in semiconductorsdoped on the metallic side of the metal-insulator transition, although this appears to havebeen verified only for the two-dimensional case, where β = 4 . It is also true that thethin implants measured in  should be close to two-dimensional.
Since a real electron heating effect would depend on power density, while normal electricfield effects depend on E, it might at first seem that we could distinguish between thesemodels by varying the sample geometry. However, a simple algebraic exercise showsthat the shape drops out and P V E= 2 ρ , so there is no way to distinguish an electric
Fig. 14. Parameters fit to the hot electron model for a number of ion-implanted Si devices.a) Best-fit power law exponent β as a function of T0. b) Ge-ph at 0.1 K as a function of T0
field effect from a power density effect without theoretical guidance. We therefore mightconsider the hot electron model simply a convenient if accidental analytic description ofR(T,E) in a range of parameters where (4), for whatever reason, does not apply.
Time constants and heat capacity. However, the hot electron picture has consequencesthat go beyond a particular R(T,E) relation. Since the electron system should have someheat capacity C e, and we have already determined an electron-phonon thermalconductivity Ge–ph, then there should be a characteristic time τ = −C Ge e ph for changes inthe electron temperature Te. This has been investigated for NTD Ge [28,29], for ionimplanted Si [32,33], and for other disordered systems [34,35]. A thermometer directlyattached to the heat sink so that its lattice temperature does not change should look like asimple bolometer as shown in Ch. 1, with the thermal link provided by Ge-ph and thebolometer heat capacity equal to Ce. This is clearly observed, and the thermal timeconstant τ can be determined quite precisely by measuring the A.C. impedance of thedevice as a function of frequency and fitting the Z(ω) function given in Ch 1. Details ofthis procedure and an example of a measurement of a “tied down” thermometer can befound in .
Figure 15 shows Ge–ph(Te) as determined from D.C. I-V curves, τ(Te) as determined fromA.C. impedance measurements, and their product, which in this hot electron pictureshould represent the heat capacity of the conduction electron system, Ce. Remarkably,while the independently-measured G e–ph and τ both vary by almost three orders ofmagnitude over this temperature range, their product is almost constant. Even moreremarkable, if one chooses to regard the hot electron model as simply an empiricaldescription of R(T,E), is that a conventional measurement of the total heat capacity of theimplanted impurity system, also shown in Fig. 15c, agrees almost perfectly with thederived Ce . This indicates that essentially all of the heat capacity of the impuritysystem is effectively coupled to the part of the system directly involved in conduction.
The electronic heat capacity, both derived and measured, is considerably flatter than thelinear temperature dependence expected for a metallic system. It is almost constantbelow 0.1 K, then steepens at higher temperatures, approaching γ = 1 at 0.2 K. This is ingood qualitative agreement with other measurements [37,38], and the small shift inabsolute value could be due to the difference in compensation (50% vs ~0%). The flattemperature dependence (which becomes negative at sufficiently low doping densities)was predicted and is ascribed to the formation of spin-exchange clusters .
Internal thermodynamic fluctuation noise. Another consequence of the literalinterpretation of the hot electron model is that additional noise should be observed in thebiased thermometer output due to transduced temperature fluctuations of the electronsystem caused by random energy transport between the electron and phonon systems.Figure 16 shows the measured noise in a “tied down” implant, after the Johnson noise ofthe resistance is subtracted. The noise and its temperature and bias dependence arereadily calculated from the simple bolometer theory outlined in Ch. 1, and the agreementis very good.
Electron Temperature (K)
This means that when a doped semiconductor thermometer is used in a bolometer orcalorimeter structure with a separate absorber and thermal isolation link, the effective“thermal circuit” must include at least two thermal links and two heat capacities. Internalthermodynamic fluctuations and internal time constants may become important. Thesimple detector theory of Ch. 1 can be used only if Ge–ph >> Gsink In general, it will benecessary to use more complicated thermal models, such as those derived in , that canexplicitly include Ge–ph and Ce.
4 Excess noise
Additional noise has been observed, primarily in ion-implanted silicon, that appears as anunexpected low-frequency component and has had a significant impact on detectorperformance. Ion implanted Si detectors made in three different labs according tosomewhat different recipes all show similar behavior . Characterization of the noiseof these thin (~200 nm) stacked-implant devices over a wide range of doping density,
Fig. 15. Measurements of ion implanted and diffused Si:P:B devices with net doping densities near2 5 1018 3. × cm- and 50% compensation (T0 ≈ 6 – 11 K). a) Coupling constant Ge–ph as a function ofTe determined from D.C. resistance as a function of bias power. b) Characteristic time constant τas a function of Te, determined from A.C. impedance measurements. c) Open symbols are theproduct of a) and b): electronic heat capacity C Ge = ⋅e– ph τ . The filled symbols are the heatcapacity of the implanted silicon measured conventionally by attaching a piece of this material to athermally isolated platform. The lines show published heat capacity measurements ofuncompensated doped Si:P with similar net donor densities from  and . (data from )
0 5 10 15 20Calculated Fluctuation Noise (nV/Hz–1/2)
m = 1.0mfit = 1.17
lattice temperature, and bias current shows a complicated dependence on all of thesefactors (including the load resistor value) . When interpreted in terms of the hotelectron model described above, however, the behavior after correcting for bias powerheating of the electrons and electrothermal feedback effects is greatly simplified and canbe characterized as relative resistance fluctuations with a 1/f spectral density that dependonly on the electron temperature and doping density. Figure 17 shows the resistancefluctuations as a function of Te for different lattice temperatures and bias currents.Combinations of these that result in the same Te also give the same derived values for
∆R R( )2.
The resistance fluctuations are independent of the shape of the device going from 36:1 to1:36 length to width ratios, which virtually rules out the ohmic contacts as a significantcontributor. They scale quite precisely with (thermistor volume)–1/2, as expected for anyrandom fluctuation that is uncorrelated in different parts of the volume. Since thethickness of these devices is limited by the acceleration energy of standard commercialion implanters, they all have approximately the same thickness. So it is actually only thearea–1/2 dependence that has been verified. The conventional parameterization for 1/fnoise is the Hooge-alpha:
2 αHooge , (6)
where N is a stand-in for the volume, and is conventionally the number of “carriers”.Han et al  arbitrarily use the net number of donors for N. Since the doping density
Fig. 16. Excess noise observed in an ion implanted Si detector tied down to the heat sink. Theobserved excess is in reasonable agreement with the predictions of standard bolometer theory forthermodynamic fluctuations over a thermal link with the measured value of Ge–ph. (from )
Fig. 16. Excess noise observed in an ion implanted Si detector tied down to the heat sink. Theobserved excess is in reasonable agreement with the predictions of standard bolometer theory forthermodynamic fluctuations over a thermal link with the measured value of Ge–ph. (from )
0.06 0.08 0.1 0.3
100mK (o5a)70.3mK (o5a)150mK (o5a)150mK (o7a)200mK (o7a)250mK (o7a)300mK (o7a)
Electron Temperature (K)
T0 = 11 K
60 mK (o5a) 90 mK (o5a)
does not change very much over the practical range of T0, this is nearly equivalent tovolume. Figure 18 shows measurements of αHooge as a function of Te for a range ofdoping densities (T0). These were reasonably well-fit by the empirical function
0 0341 0
2 453 5 2 0 9 110 0
., ( . . log ( /
There has been only a little theoretical work on fluctuations in hopping conductivity[43,44], and it is not clear that what has been done is applicable to the usual conditionsfor low-temperature thermometers. It can be seen from Fig. 18 that the 1/f noiseincreases rapidly as Te decreases, going approximately as Te
–6. Perhaps coincidentally,the size of the percolation network at these temperatures is becoming comparable to thedevice thickness and is increasing exponentially as the temperature drops, making theconduction rapidly more two-dimensional . Thus the strong temperature dependenceoffers a hint that the 1/f noise is a 2-d or surface effect. NTD Ge thermometers generallydo not show significant 1/f noise, but most Ge devices are at least 100 µm thick, and thereare at least anecdotal reports of it showing up in unusually thin Ge.
The ready availability of good quality silicon-on-insulator wafers with almost any desireddevice thickness now makes it straightforward to fabricate thicker doped Sithermometers. As described in , these have been made by implanting the phosphorus
Fig. 17. Resistance fluctuations in a thin ion-implanted Si thermometer as a function of theelectron temperature Te for several values of Tlattice and bias. The fluctuations appear to dependonly on Te, which increases with bias power for a given Tlattice. (from )
0.04 0.06 0.08 0.1 0.3
Electron Temperature (K)
43 K25 K
11 K4.8 K
and boron dopants at approximately the middle of a 1.5 µm silicon layer, then annealingat high temperature for a long time so that the impurity atoms diffuse uniformly throughthe entire thickness. The 1/f noise in these devices is reduced by at least a factor of six,as shown in Fig. 19.
10 100 1000 10000
Predicted Measured Bias V
Fig. 18. Excess noise parameter αHooge for thermistors with different doping densities.
Fig. 19. Noise spectra from a 1500 nm thick diffused implant in Si. The lines show thepredictions from (7). In the absence of 1/f noise, the white noise level falls with increasingbias due to the drop in resistance from bias power heating of the electrons. (from )
An alternative explanation for the 1/f noise is that while it is a surface effect, it is causedby the proximity of the lightly-doped wings of the stacked-implant profile . Slowtunneling of electrons between sites that are not part of the conduction network couldmodulate the main conduction path, in analogy to the standard McWhorter theory of lowfrequency noise in Metal-Oxide-Semiconductor Field Effect Transistors. Theimprovement is then due less to the increased thickness than to the very abrupt cutoff inthe doping density profile. There are obvious experiments that could distinguish betweenthese possibilities, but they have not been done.
5 Fundamental Limitations and Ultimate Performance
The “non-ideal” effects described above all limit the performance of detectors withsemiconductor thermometers. The linear analysis of Ch. 1 gives the logarithmicsensitivity α as the only significant thermometer parameter. Hot electron and fieldeffects limit practical values of α to 10 or less in most cases — far less than thesensitivity currently available with superconducting transition edge thermistors. So whyuse semiconductors at all? The answer to this is certainly application-dependent. Themost obvious consideration is large signals, where the saturation characteristics oftransition edge sensors are best described as “less than graceful.” Semiconductorthermometers become more nonlinear and less sensitive with increasing signal size, buthave no hard saturation limits. They are easier to characterize and can also be easier tofabricate and simpler to use. The ideal amplifier for semiconductor thermometers is asimple Junction Field Effect Transistor (JFET) costing less than $1. On the other hand,for large numbers of detectors practical advantage can swing strongly in favor of theSQUID amplifiers used with superconducting thermometers.
One perhaps fundamental advantage of semiconductors is that they are relativelyinsensitive to magnetic fields. They have been operated without degradation in fields aslarge as 10 T . The characteristics shift considerably, but the thermometer can beoptimized for a given field. Conversely, a single thermometer can be made to performover a wide range of temperatures by “tuning” it with a variable magnetic field.
Even the shortcomings can occasionally be put to good use. The hot electron effectallows a simple thermometer to be used as a complete detector, with an absoluteminimum of addenda. The electron system is both the absorber and the thermometer, andthe thermal isolation suspension is provided by the electron-phonon coupling. The usualdrawback of these hot electron bolometers is that they have few adjustable parametersand cannot be optimized for a particular situation. However, the built-in characteristicsof thin silicon implants are almost ideal for the requirements of some infrared detectorapplications [48,49]. The R.F. sheet resistance is a good match to free space or a simpletransmission line, so the absorber is highly efficient. Time constants cover a reasonablerange at temperatures where the thermodynamic performance is good, and the low-frequency resistance for a square detector is a good match to the noise resistance of aJFET amplifier. It appears that very simple detectors could be made with outstandingperformance.
Getting the best possible performance requires optimizing the thermometer design. Todo this, one needs both an understanding of how the thermometer works and quantitativedata on the behavior of key parameters. We now seem to have an adequatephenomenological understanding of how semiconductor thermometers work, even if theunderlying theory is a little murky. The hot electron model should be taken at face valueand modeled as a separate thermal conductance and heat capacity. This complicates thethermal circuit (aside from the happy case of the hot electron bolometer) but appears toaccount correctly for the additional time constants and noise sources that are observed,and formalisms exist for handling arbitrary thermal models [40,50]. The field effect canbe included simultaneously. In the linearized performance theory of Ch. 1 it shows up asthe parameter β ∂ ∂≡ )log logR V
T. For the field effect model (4), β is simply
−CeE kTλ . Of course, to perform the optimization, one has to know how β, Ge–ph, and Ce
depend on other parameters.
We are not so well off with the necessary engineering data. The data for silicon arebarely adequate for low T0 material operated at not too low temperatures where electricfield effects are negligible. For NTD germanium both field effect and electron heatingare usually important, and there is a surprising scarcity data on either. Part of theproblem is that little analysis has been done that takes both effects into account, and thishas confused the results. Now that the situation is better understood, it is relatively easyto separate parameters and evaluate both effects simultaneously. It is straightforward tomeasure the A.C. impedance Z( )ω , and since β = − ∞1 R Z/ ( ) , β and with it the localvalue of λ can be extracted immediately from its high frequency limit. This can be usedto separate heating and field effects at the bias point, giving a value for Ge–ph, which alongwith β can then be put into the fit of Z( )ω to get τ and Ce.
5.2 Germanium vs Silicon
The choice of Si or Ge depends very much on the application, and is usually decided bynon-performance characteristics such as the excellent reproducibility of NTD Ge or theease of fabricating large numbers of small integrated thermometers with ion-implantedSi. However, it is still interesting to consider whether there is some universal figure ofmerit that favors one or the other. The beneficial thermometer parameter is its sensitivity,while its heat capacity has a negative impact on detector performance. Both electric fieldand hot electron effects reduce the effective sensitivity as the power density goes up anda rough figure of merit would be sensitivity at a given power per unit heat capacity andtemperature. This is a complex quantity, since field effect and electron heating affect thesensitivity in different ways.
Field effect (non-zero β) reduces both signal and thermodynamic fluctuation noise by thesame amount, so if amplifier noise is not significant, the only change in signal to noiseratio comes from Johnson noise. Johnson noise in biased nonlinear resistances is adiffiicult theoretical subject [51,52] that we will avoid here, since hot electrons generallyhave more impact on detector performance than field effect. (The opposite is the case forsuperconducting transition edge thermometers, so see the next chapter for morediscussion.) In the usual case where the signal comes in through the phonon system, the
sensitivity to phonon temperature is rapidly degraded by electron heating. This can beseen from (5), remembering that the exponent is ~6. The thermodynamic fluctuationsbetween the electron and phonon baths can create additional noise, and the C Ge e ph− timeconstant rolls off the signal spectrum with respect to the thermometer Johnson noise andwill degrade the overall signal to noise ratio unless it is shorter than the primary thermaltime constant of the detector by a factor of ~α. For all of these hot electron effects, thefigure of merit is G Cee ph− at a given thermometer sensitivity α ≈ 0 5 0
1 2. ( / )T T . Thisquantity is independent of thermometer volume, and is plotted in Fig. 20 asτ e ph e ph− −≡ C Ge . Data for NTD Ge are very sparse and inconsistent by a factor of ten ormore. On the average, however, it appears that the intrinsic time constants may be fasterby a factor of about six for the same T0 and Te. Much better data are needed for designoptimization and predictions of ultimate performance, and it should be straightforward tomake the necessary measurements.
5.3 Expected performance
We are at a point where performance can be predicted with reasonable accuracy whenthermal data are available. A 32-detector array, identical to the XRS-2 array shown inFig. 8, was built for an atomic physics experiment and operated at 60 mK. It hadmeasured resolution within 10% of the calculated 4.8 eV F.W.H.M. for 6 keV X-rays on(almost) all of the detectors. Given the particular X-ray absorber used, the main avenuefor improving the resolution would be to improve the thermal coupling between theabsorber and thermistors. With perfect coupling, the predicted resolution would be3.4 eV, but problems with “thermalization noise”, where variable numbers of super-thermal phonons reaching the thermometer produce pulse-to-pulse variations in theresponse, would actually make the resolution worse. The optimum solution for this is
T0 = 1 K
T0 = 5 K
T0 = 10 K
T0 = 20 K
T0 = 40 K
T0 = 60 K
Fig. 20. The electron-phonon time constant C Ge e ph− vs electron temperature. The solid lines
are for Si with doping density given by the indicated T0 using fits to Ge ph− data from  with
normalization and Ce from 
unknown, and the phonon physics is complex, so progress requires experimenting withdifferent absorber couplings. Lowering the operating temperature could improve theresolution further, and germanium thermometers might be better, but we don’t have thedata to say by how much or under what conditions.
One of the better X-ray detector results obtained so far with a semiconductorthermometer is shown in Fig. 21. There is some room for improvement: one mightexpect that if everything could be optimized, a 2 eV detector with these parameters isfeasible. But for a detector of this heat capacity operating at ~50 mK, some otherthermometer technology will be necessary to reach 1 eV.
5870 5880 5890 5900 5910 5920
Intrinsic Mn K 1,2 profile
Fit: 3.2 ± 0.1 eV FWHM
Pulse Height (eV)
I would like to thank E.E. Haller and J.W. Beeman for providing their data on NTD Geprior to publication. Many members of the Wisconsin and NASA/Goddard X-ray groupscontributed heavily to this chapter. I thank in particular Jiahong Zhang, Mike Juda,Massimiliano Galleazzi, Andy Szymkowiak, Scott Porter, Caroline Kilbourne, RichardKelley, and Regis Brekosky. This work was supported in part by NASA grant NAG5-5404.
Fig. 21. Pulse height spectrum of the 55Mn Kα1 and Kα2 lines at 5.9 keV, showing a resolutionof 3.2 ± 0.1 eV FWHM. This device had a uniformly illuminated 0.41 x 0.41 mm2 HgTeabsorber 8 µm thick, which provides better than 95% X-ray stopping efficiency up to 7 keV and50% up to 17 keV. It was operated at a detector temperature of ~60 mK
1. R. C. Jones, J. Opt. Soc. Am. 37, 879 (1947) 2. I. Esterman, Phys. Rev. 78, 83 (1950) 3. F. J. Low, J. Opt. Soc. Am. 51, 1300 (1961) 4. P.W. Anderson, phys. Rev. 109, 1492 (1958) 5. N.F. Mott & W.D. Twose, Adv. Phys. 10, 107 (1961) 6. B.I. Shklovskii & A.L. Efros, Electronic Properties of Doped Semiconductors
(Springer, Berlin 1984) 7. A.L. Efros & B.I. Shklovskii, J. Phys. C 8, L49 (1975) 8. J. Zhang et al., Phys. Rev. B 48, 2312 (1993) 9. J. Zhang et al., Phys. Rev. B 57, 4950 (1998; erratum to )10. I.S. Shlimak, in Hopping and Related Phenomena eds. H. Fritzsche & M. Pollak
(World Scientific, Singapore 1990) p. 4911. P. Dai, Y. Zhang, & M.P. Sarachik, Phys. Rev. Lett. 69, 1804 (1992)12. W. Bergmann-Tiest, personal communication (1998)13. L.R. Semo-Scharfman, personal communication (2003)14. A.L. Woodcraft et al., J. Low Temp. Phys. 134, 925 (2004)15. E.E. Haller, N.P. Palaio, M. Rodder, W.L. Hansen, and E. Kreysa, in Neutron
Transmutation Doping of Semiconductor Materials, ed. R.D. Larrabee (Plenum,New York 1984) p 21
16. Itoh et al., J. Low Temp. Phys. 93, 307 (1993)17. E. E. Haller & J.W. Beeman, personal communication (2004)18. C. Arnaboldi et al., Nucl. Instr. Methods A518, 775 (2004)19. A.D. Turner et al., Appl. Optics 40, 4921 (2001)20. R.P. Brekosky et al., Nucl. Instr. & Methods A520, 439 (2004)21. P.M. Downey et al., Appl. Optics 23, 910 (1984)22, S.H. Moseley, J.C. Mather, & D. McCammon, J. Appl. Phys. 56, 1257 (1984)23. R.M. Hill, Philos. Mag. 24, 1307 (1971)24. J. Zhang et al., Phys. Rev. B 57, 4472 (1998)25. T.W. Kenny et al., Phys. Rev. B 39, 8476 (1989)26. S.M. Grannan, A.E. Lange, E.E. Haller, and J.W. Beeman, Phys. Rev. B 45, 4516
(1992)27. M. Piat et al., J. Low Temp. Phys. 125, 189 (2001)28. N. Wang et al., Phys. Rev. B 41, 3761 (1990)29. E. Auberg et al., J. Low Temp. Phys. 93, 289 (1993)30. B.I. Shklovskii, personal communication (2004)31. M. Prunnila et al, Physica E 13, 773 (2002)32. D. Liu et al., in Low Temperature Detectors, (F.S. Porter et al. Eds.), Proc. 9th Int'l
Workshop on Low Temperature Detectors in Madison, Wisconsin, July 2001 (AIP,New York 2002) p 87. (see also M. Galeazzi et al., Nucl. Instr. Methods A 420, 469(2004))
33. M. Galeazzi et al., Phys. Rev. B (submitted)34. M.A. LaMadrid, W. Contrata, J.M. Mochel, Phys. Rev. B 45, 3870 (1992)35. S. Marnieros, L. Bergé, A. Juillard, & L. Dumoulin, Phys. Rev. Lett. 84, 2469 (2000)
36. J.E. Vaillancourt, Rev. Sci. Instr. (in press)37. M.A. Paalanen, J.E. Graebner, R.N. Bhatt, Phys. Rev. Lett. 61, 597 (1988)38. M. Lakner, H.v. Löhneysen, Phys. Rev. Lett. 63, 648 (1989)39. R.N. Bhatt, P.A. Lee, Phys. Rev. Lett. 48, 344 (1982)40. M. Galeazzi, D. McCammon, J. Appl. Phys. 93, 4856 (2003)41. A. Nucciotti, personal communication (1998)42. S-I Han et al., in EUV, X-Ray and Gamma-Ray Instrumentation for Astronomy IX,
(O.H. Siegmund, M.A. Gummin, Eds.), Proc. SPIE v.3445, 640 (1998)43. B.I. Shklovskii, Solid State Commun. 33, 273 (1980)44. Sh.M. Kogan, B.I. Shklovskii, Fiz. Tekh. Poluprovodn. 15, 1049 (1981) [Sov. Phys.
Semicond. 15, 605 (1981)]45. D. McCammon et al., in Low Temperature Detectors, (F.S. Porter et al. Eds.), Proc.
9th Int'l Workshop on Low Temperature Detectors in Madison, Wisconsin, July2001 (AIP, New York 2002) p 91
46. S.H. Moseley, personal communication (2001)47. P. De Moor et al., J Low Temp. Phys. 93, 295 (1993)48. H. Moseley, D. McCammon, in Low Temperature Detectors, (F.S. Porter et al. Eds.),
Proc. 9th Int'l Workshop on Low Temperature Detectors in Madison, Wisconsin,July 2001 (AIP, New York 2002) p 103
49. T.R. Stevenson et al., in Millimeter and Submillimeter Detectors for Astronomy II,(J. Zmuidzinas, W.S. Holland Eds.), Proc. SPIE v.5498 (in press)
50. E. Figueroa-Feliciano, Ph.D. thesis, Stanford University (2001)51. H.B. Callen & T.A. Welton, Phys. Rev. 83, 34 (1951)52. L. Weiss & W. Mathis, IEEE Electron Device Lett. 20, 402 (1999)